LMucko/crystallography-open-database huggingface dataset:
Crystal structure and ligand mobility in solution ofcis-dimethyl-bis(trimethylphosphine)gold(III) complexes
Schuster, O.; Schmidbaur, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 61 (2006) 1–5; doi:

data_7221508
_publ_section_title
;
 Crystal structure and ligand mobility in solution
 ofcis-dimethyl-bis(trimethylphosphine)gold(III) complexes
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1
_journal_page_last               5
_journal_volume                  61
_journal_year                    2006
_chemical_formula_sum            'C9 H26 Au Cl3 O4 P2'
_chemical_name_systematic        '(C H3)2 Au (P (C H3)3)2 Cl O4 (C H2 Cl2)'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.1865
_cell_length_b                   17.6364
_cell_length_c                   8.1742
_cell_volume                     1901.011
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Schuster_ZNBSEN_2006_796.cif
_cod_data_source_block           C9H26Au1Cl3O4P2
_cod_original_formula_sum        'C9 H26 Au1 Cl3 O4 P2'
_cod_database_code               7221508
Crystal structure and ligand mobility in solution ofcis-dimethyl-bis(trimethylphosphine)gold(III) complexes
Schuster, O.; Schmidbaur, H.; Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische Chemie (42,1987-) 61 (2006) 1–5; doi:

data_7221509
_publ_section_title
;
 Crystal structure and ligand mobility in solution
 ofcis-dimethyl-bis(trimethylphosphine)gold(III) complexes
;
_journal_name_full
;
Zeitschrift fuer Naturforschung, Teil B. Anorganische Chemie, Organische 
Chemie (42,1987-)
;
_journal_page_first              1
_journal_page_last               5
_journal_volume                  61
_journal_year                    2006
_chemical_formula_sum            'C8 H24 Au I P2'
_chemical_name_systematic        '(C H3)2 Au (P (C H3)3)2 I'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.6285
_cell_length_b                   19.771
_cell_length_c                   7.6701
_cell_volume                     1763.410
_citation_journal_id_ASTM        ZNBSEN
_cod_data_source_file            Schuster_ZNBSEN_2006_797.cif
_cod_data_source_block           C8H24Au1I1P2
_cod_original_cell_volume        1763.41
_cod_original_formula_sum        'C8 H24 Au1 I1 P2'
_cod_database_code               7221509
Synthesis and crystal structures of novel copper(I) complexes of a phosphanylborane
Schwan, K.C.; Adolf, A.; Scheer, M.; Bodensteiner, M.; Zabel, M.; Zeitschrift fuer Anorganische und Allgemeine Chemie 634 (2008) 1383–1387; doi:

data_1528860
_publ_section_title
;
 Synthesis and crystal structures of novel copper(I) complexes of a
 phosphanylborane
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              1383
_journal_page_last               1387
_journal_volume                  634
_journal_year                    2008
_chemical_formula_sum            'C9 H39 B3 Cu3 I3 N3 P3'
_chemical_name_systematic        'Cu3 (I)3 (P H2 B H2 N (C H3)3)3'
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 96.538
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.933
_cell_length_b                   9.429
_cell_length_c                   14.276
_cell_volume                     1462.103
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Schwan_ZAACAB_2008_1501.cif
_cod_data_source_block           C9H39B3Cu3I3N3P3
_cod_database_code               1528860
Crystal structure of Li6 Be F4 Zr F8
Sears, D.R.; Burns, J.H.; Journal of Chemical Physics 41 (1964) 3478–3483; doi:

data_1528861
_publ_section_title
;
 Crystal structure of Li6 Be F4 Zr F8
;
_journal_name_full               'Journal of Chemical Physics'
_journal_page_first              3478
_journal_page_last               3483
_journal_volume                  41
_journal_year                    1964
_chemical_formula_sum            'Be F12 Li6 Zr'
_chemical_name_systematic        'Li6 Be F4 Zr F8'
_space_group_IT_number           141
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.57
_cell_length_b                   6.57
_cell_length_c                   18.62
_cell_volume                     803.730
_citation_journal_id_ASTM        JCPSA6
_cod_data_source_file            Sears_JCPSA6_1964_1776.cif
_cod_data_source_block           Be1F12Li6Zr1
_cod_original_cell_volume        803.7305
_cod_original_formula_sum        'Be1 F12 Li6 Zr1'
_cod_database_code               1528861
Das Strukturprinzip des Strontiumvanadat, Sr (V O3)2 (H2 O)4
Sedlacek, P.; Dornberger-Schiff, K.; Acta Crystallographica (1,1948-23,1967) 18 (1965) 407–410; doi:

data_2310661
_publ_section_title
;
 Das Strukturprinzip des Strontiumvanadat, Sr (V O3)2 (H2 O)4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              407
_journal_page_last               410
_journal_volume                  18
_journal_year                    1965
_chemical_formula_sum            'H8 O10 Sr V2'
_chemical_name_systematic        'Sr (V O3)2 (H2 O)4'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2n 2a'
_symmetry_space_group_name_H-M   'P m c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.38
_cell_length_b                   33.6
_cell_length_c                   7.16
_cell_volume                     1775.451
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Sedlacek_ACCRA9_1965_1870.cif
_cod_data_source_block           H8O10Sr1V2
_cod_original_sg_symbol_Hall     '-P 2ac 2n (y,z,x)'
_cod_original_formula_sum        'H8 O10 Sr1 V2'
_cod_database_code               2310661
Die Kristallstruktur des Lithiummetasilikates, (Li2 Si O3)x
Seemann, H.; Acta Crystallographica (1,1948-23,1967) 9 (1956) 251–252; doi:

data_2310662
_publ_section_title
;
 Die Kristallstruktur des Lithiummetasilikates, (Li2 Si O3)x
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              251
_journal_page_last               252
_journal_volume                  9
_journal_year                    1956
_chemical_formula_sum            'Li2 O3 Si'
_chemical_name_systematic        'Li2 (Si O3)'
_space_group_IT_number           36
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.36
_cell_length_b                   5.395
_cell_length_c                   4.675
_cell_volume                     236.074
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Seemann_ACCRA9_1956_189.cif
_cod_data_source_block           Li2O3Si1
_cod_original_cell_volume        236.0744
_cod_original_formula_sum        'Li2 O3 Si1'
_cod_database_code               2310662
A refinement of zinc dichloride-hydrochloric acid-water (2:1:2)
Selenius, C.O.; Delaplane, R.G.; Acta Crystallographica B (24,1968-38,1982) 34 (1978) 1330–1332; doi:

data_2106587
_publ_section_title
;
 A refinement of zinc dichloride-hydrochloric acid-water (2:1:2)
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              1330
_journal_page_last               1332
_journal_volume                  34
_journal_year                    1978
_chemical_formula_sum            'Cl5 H5 O2 Zn2'
_chemical_name_systematic        '(Zn Cl2)2 (H Cl) (H2 O)2'
_space_group_IT_number           43
_symmetry_space_group_name_Hall  'F 2 -2d'
_symmetry_space_group_name_H-M   'F d d 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   9.243
_cell_length_b                   22.885
_cell_length_c                   8.886
_cell_volume                     1879.621
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Selenius_ACBCAR_1978_507.cif
_cod_data_source_block           H5Cl5O2Zn2
_cod_original_cell_volume        1879.62
_cod_original_formula_sum        'H5 Cl5 O2 Zn2'
_cod_database_code               2106587
The crystal structures of Nb3 Se4 and Nb3 Te4
Selte, K.; Kjekshus, A.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 1568–1572; doi:

data_2310663
_publ_section_title
;
 The crystal structures of Nb3 Se4 and Nb3 Te4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              1568
_journal_page_last               1572
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Nb3 Te4'
_space_group_IT_number           176
_symmetry_space_group_name_Hall  '-P 6c'
_symmetry_space_group_name_H-M   'P 63/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   10.671
_cell_length_b                   10.671
_cell_length_c                   3.6468
_cell_volume                     359.627
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Selte_ACCRA9_1964_177.cif
_cod_data_source_block           Nb3Te4
_cod_original_cell_volume        359.6274
_cod_database_code               2310663
The Structure of Synthetic Copper Sodium Phosphate: Cu9 Na6 (P O4)8
Senga, Y.; Kawahara, A.; Acta Crystallographica B (24,1968-38,1982) 36 (1980) 2555–2558; doi:

data_2106588
_publ_section_title
;
 The Structure of Synthetic Copper Sodium Phosphate: Cu9 Na6 (P O4)8
;
_journal_name_full               'Acta Crystallographica B (24,1968-38,1982)'
_journal_page_first              2555
_journal_page_last               2558
_journal_volume                  36
_journal_year                    1980
_chemical_formula_sum            'Cu9 Na6 O32 P8'
_chemical_name_systematic        'Cu9 Na6 (P O4)8'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                102.25
_cell_angle_beta                 100.2
_cell_angle_gamma                113.1
_cell_formula_units_Z            1
_cell_length_a                   9.3069
_cell_length_b                   8.9152
_cell_length_c                   8.7838
_cell_volume                     627.041
_citation_journal_id_ASTM        ACBCAR
_cod_data_source_file            Senga_ACBCAR_1980_64.cif
_cod_data_source_block           Cu9Na6O32P8
_cod_original_cell_volume        627.0413
_cod_database_code               2106588
Die Koordinationszahl 5 bei Rb Nb O3: Eine Pyrgomstruktur
Serafin, M.; Hoppe, R.; Naturwissenschaften 66 (1979) 50–51; doi:

data_1528862
_publ_section_title
;
 Die Koordinationszahl 5 bei Rb Nb O3: Eine Pyrgomstruktur
;
_journal_name_full               Naturwissenschaften
_journal_page_first              50
_journal_page_last               51
_journal_volume                  66
_journal_year                    1979
_chemical_formula_sum            'Nb O3 Rb'
_chemical_name_systematic        'Rb Nb O3'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                94.6
_cell_angle_beta                 93.5
_cell_angle_gamma                113.9
_cell_formula_units_Z            4
_cell_length_a                   8.87
_cell_length_b                   8.39
_cell_length_c                   5.11
_cell_volume                     344.725
_citation_journal_id_ASTM        NATWAY
_cod_data_source_file            Serafin_NATWAY_1979_18.cif
_cod_data_source_block           Nb1O3Rb1
_cod_original_cell_volume        344.7245
_cod_original_formula_sum        'Nb1 O3 Rb1'
_cod_database_code               1528862
Synthesis and x-ray structural investigation of K8 [(U O2) (C2 O4)2 (Se O4)4] * 2 H2 O
Serezhkina, L.B.; Verevkin, A.G.; Peresypkina, E.V.; Virovets, A.; Pushkin, D.V.; Kristallografiya 54 (2009) 68–71; doi:

data_1528863
_publ_section_title
;
 Synthesis and x-ray structural investigation of K8 [(U O2) (C2 O4)2 (Se
 O4)4] * 2 H2 O
;
_journal_name_full               Kristallografiya
_journal_page_first              68
_journal_page_last               71
_journal_volume                  54
_journal_year                    2009
_chemical_formula_sum            'C4 H4 K8 O30 Se4 U2'
_chemical_name_systematic        'K8 ((U O2)2 (C2 O4)2 (Se O4)4) (H2 O )2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.188
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.929
_cell_length_b                   7.28
_cell_length_c                   15.3165
_cell_volume                     1572.166
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Serezhkina_KRISAJ_2009_1666.cif
_cod_data_source_block           C4H4K8O30Se4U2
_cod_original_sg_symbol_Hall     '-P 2ybc (x-z,y,z)'
_cod_database_code               1528863
Co8 (C O)24 C6, a bis(tricobalt nonacarbonyl) dicobalt hexacarbonyl derivative of 2,4-hexadiyne from the reaction of dicobalt octacarbonyl with hexachlorocyclopropane
Seyferth, D.; Spohn, R.J.; Churchill, M.R.; Gold, K.; Scholer, F.R.; Journal of Organometallic Chemistry 23 (1970) 237–255; doi:

data_4031265
_publ_section_title
;
 Co8 (C O)24 C6, a bis(tricobalt nonacarbonyl) dicobalt hexacarbonyl
 derivative of 2,4-hexadiyne from the reaction of dicobalt octacarbonyl
 with hexachlorocyclopropane
;
_journal_name_full               'Journal of Organometallic Chemistry'
_journal_page_first              237
_journal_page_last               255
_journal_volume                  23
_journal_year                    1970
_chemical_formula_sum            'C33 H3 Co8 O24'
_chemical_name_systematic        'Co8 (C O)24 C6 (C6 H6)0.5'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                99.78
_cell_angle_beta                 115.06
_cell_angle_gamma                74.39
_cell_formula_units_Z            2
_cell_length_a                   15.57
_cell_length_b                   16.32
_cell_length_c                   8.77
_cell_volume                     1940.248
_citation_journal_id_ASTM        JORCAI
_cod_data_source_file            Seyferth_JORCAI_1970_122.cif
_cod_data_source_block           C33H3Co8O24
_cod_database_code               4031265
Nanocrystalline Na Nb O3 and Na Ta O3: Rietveld studies, Raman spectroscopy and dielectric properties
Shanker, V.; Samal, S.L.; Narayana, C.; Pradhan, G.K.; Ganguli, A.K.; Solid State Sciences 11 (2009) 562–569; doi:

data_1528864
_publ_section_title
;
 Nanocrystalline Na Nb O3 and Na Ta O3: Rietveld studies, Raman
 spectroscopy and dielectric properties
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              562
_journal_page_last               569
_journal_volume                  11
_journal_year                    2009
_chemical_formula_sum            'Na Nb O3'
_chemical_name_systematic        'Na (Nb O3)'
_space_group_IT_number           26
_symmetry_space_group_name_Hall  'P 2c -2'
_symmetry_space_group_name_H-M   'P m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.8636
_cell_length_b                   5.6306
_cell_length_c                   5.5483
_cell_volume                     245.661
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Shanker_SSSCFJ_2009_1672.cif
_cod_data_source_block           Na1Nb1O3
_cod_original_cell_volume        245.6609
_cod_original_formula_sum        'Na1 Nb1 O3'
_cod_database_code               1528864
Nanocrystalline Na Nb O3 and Na Ta O3: Rietveld studies, Raman spectroscopy and dielectric properties
Shanker, V.; Samal, S.L.; Pradhan, G.K.; Narayana, C.; Ganguli, A.K.; Solid State Sciences 11 (2009) 562–569; doi:

data_1528865
_publ_section_title
;
 Nanocrystalline Na Nb O3 and Na Ta O3: Rietveld studies, Raman
 spectroscopy and dielectric properties
;
_journal_name_full               'Solid State Sciences'
_journal_page_first              562
_journal_page_last               569
_journal_volume                  11
_journal_year                    2009
_chemical_formula_sum            'Na O3 Ta'
_chemical_name_systematic        'Na (Ta O3)'
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.5883
_cell_length_b                   5.6584
_cell_length_c                   7.9309
_cell_volume                     250.782
_citation_journal_id_ASTM        SSSCFJ
_cod_data_source_file            Shanker_SSSCFJ_2009_1673.cif
_cod_data_source_block           Na1O3Ta1
_cod_original_cell_volume        250.7817
_cod_original_sg_symbol_Hall     '-P 2ac 2n (z,x,y)'
_cod_original_formula_sum        'Na1 O3 Ta1'
_cod_database_code               1528865
The structures of the reduced and oxidized forms of barium silicon tantalum oxide Ba3 Si4 Ta6 O23 and Ba3 Si4 Ta6 O26
Shannon, J.; Katz, L.; Journal of Solid State Chemistry 1 (1970) 399–408; doi:

data_1528866
_publ_section_title
;
 The structures of the reduced and oxidized forms of barium silicon
 tantalum oxide Ba3 Si4 Ta6 O23 and Ba3 Si4 Ta6 O26
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              399
_journal_page_last               408
_journal_volume                  1
_journal_year                    1970
_chemical_formula_sum            'Ba3 O23 Si4 Ta6'
_chemical_name_systematic        'Ba3 Si4 Ta6 O23'
_space_group_IT_number           189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.997
_cell_length_b                   8.997
_cell_length_c                   7.745
_cell_volume                     542.935
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Shannon_JSSCBI_1970_1926.cif
_cod_data_source_block           Ba3O23Si4Ta6
_cod_original_cell_volume        542.9345
_cod_database_code               1528866
The structures of the reduced and oxidized forms of barium silicon tantalum oxide Ba3 Si4 Ta6 O23 and Ba3 Si4 Ta6 O26
Shannon, J.; Katz, L.; Journal of Solid State Chemistry 1 (1970) 399–408; doi:

data_1528867
_publ_section_title
;
 The structures of the reduced and oxidized forms of barium silicon
 tantalum oxide Ba3 Si4 Ta6 O23 and Ba3 Si4 Ta6 O26
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              399
_journal_page_last               408
_journal_volume                  1
_journal_year                    1970
_chemical_formula_sum            'Ba3 O26 Si4 Ta6'
_chemical_name_systematic        'Ba3 Si4 Ta6 O26'
_space_group_IT_number           189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   8.99
_cell_length_b                   8.99
_cell_length_c                   7.79
_cell_volume                     545.240
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Shannon_JSSCBI_1970_1927.cif
_cod_data_source_block           Ba3O26Si4Ta6
_cod_original_cell_volume        545.2397
_cod_database_code               1528867
Refinement of the crystal structure of low temperature Li3 V O3 and analysis of mean bond lengths in phosphates, arsenates, and vanadates
Shannon, R.D.; Calvo, C.; Journal of Solid State Chemistry 6 (1973) 538–549; doi:

data_1528868
_publ_section_title
;
 Refinement of the crystal structure of low temperature Li3 V O3 and
 analysis of mean bond lengths in phosphates, arsenates, and vanadates
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              538
_journal_page_last               549
_journal_volume                  6
_journal_year                    1973
_chemical_formula_sum            'Li3 O4 V'
_chemical_name_systematic        'Li3 V O4'
_space_group_IT_number           31
_symmetry_space_group_name_Hall  'P 2ac -2'
_symmetry_space_group_name_H-M   'P m n 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.3259
_cell_length_b                   5.446
_cell_length_c                   4.9469
_cell_volume                     170.425
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Shannon_JSSCBI_1973_1984.cif
_cod_data_source_block           Li3O4V1
_cod_original_cell_volume        170.4249
_cod_original_formula_sum        'Li3 O4 V1'
_cod_database_code               1528868
Atomic Coordinates of Al P O4
Sharan, B.; Dutta, B.N.; Acta Crystallographica (1,1948-23,1967) 17 (1964) 82–85; doi:

data_2310664
_publ_section_title
;
 Atomic Coordinates of Al P O4
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              82
_journal_page_last               85
_journal_volume                  17
_journal_year                    1964
_chemical_formula_sum            'Al O4 P'
_chemical_name_systematic        'Al P O4'
_space_group_IT_number           152
_symmetry_space_group_name_Hall  'P 31 2"'
_symmetry_space_group_name_H-M   'P 31 2 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   4.941
_cell_length_b                   4.941
_cell_length_c                   10.95
_cell_volume                     231.513
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Sharan_ACCRA9_1964_131.cif
_cod_data_source_block           Al1O4P1
_cod_original_cell_volume        231.5125
_cod_original_formula_sum        'Al1 O4 P1'
_cod_database_code               2310664